• Study Resource
• Explore

Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

Theoretical and experimental justification for the Schrödinger equation wikipedia, lookup

Electron scattering wikipedia, lookup

Compact Muon Solenoid wikipedia, lookup

Photoelectric effect wikipedia, lookup

Electron wikipedia, lookup

Monte Carlo methods for electron transport wikipedia, lookup

Atomic nucleus wikipedia, lookup

Introduction to quantum mechanics wikipedia, lookup

Transcript
```Overview of Silicon Semiconductor
Device Physics
Dr. David W. Graham
West Virginia University
Lane Department of Computer Science and Electrical Engineering
1
Silicon
Silicon is the primary semiconductor used in VLSI systems
Si has 14 Electrons
Energy Bands
(Shells)
Valence Band
Nucleus
Silicon has 4 outer shell /
valence electrons
At T=0K, the
highest energy
band occupied by
an electron is
called the valence
band.
2
Energy Bands
}
Increasing
Electron
Energy
}
Disallowed
Energy
States
Allowed
Energy
States
• Electrons try to
occupy the lowest
energy band possible
• Not every energy
level is a legal state
for an electron to
occupy
• These legal states
tend to arrange
themselves in bands
Energy Bands
3
Energy Bands
EC
Conduction Band
First unfilled energy
band at T=0K
Eg
EV
Energy
Bandgap
Valence Band
Last filled energy
band at T=0K
4
Band Diagrams
Increasing electron energy
EC
Eg
EV
Increasing voltage
Band Diagram Representation
Energy plotted as a function of position
EC  Conduction band
 Lowest energy state for a free electron
EV  Valence band
 Highest energy state for filled outer shells
EG  Band gap
 Difference in energy levels between EC and EV
 No electrons (e-) in the bandgap (only above EC or below EV)
 EG = 1.12eV in Silicon
5
Intrinsic Semiconductor
Silicon has 4 outer shell /
valence electrons
Forms into a lattice structure
to share electrons
6
Intrinsic Silicon
The valence band is full, and
no electrons are free to move
EC
EV
However, at temperatures
above T=0K, thermal energy
shakes an electron free
7
Semiconductor Properties
For T > 0K
Electron shaken free and can
cause current to flow
h+
e–
• Generation – Creation of an electron (e-)
and hole (h+) pair
• h+ is simply a missing electron, which
leaves an excess positive charge (due to
an extra proton)
• Recombination – if an e- and an h+ come
in contact, they annihilate each other
• Electrons and holes are called “carriers”
because they are charged particles –
when they move, they carry current
• Therefore, semiconductors can conduct
electricity for T > 0K … but not much
current (at room temperature (300K), pure
silicon has only 1 free electron per 3
trillion atoms)
8
Doping
• Doping – Adding impurities to the silicon
crystal lattice to increase the number of
carriers
• Add a small number of atoms to increase
either the number of electrons or holes
9
Periodic Table
Column 3
Elements have 3
electrons in the
Valence Shell
Column 4
Elements have 4
electrons in the
Valence Shell
Column 5
Elements have 5
electrons in the
Valence Shell
10
Donors n-Type Material
•
•
•
•
•
•
•
•
Donors
electrons
ex. Phosphorous (P)
“Donates” an extra e- that can freely
travel around
Leaves behind a positively charged
nucleus (cannot move)
Overall, the crystal is still electrically
neutral
negative carriers)
ND = the concentration of donor
atoms [atoms/cm3 or cm-3]
~1015-1020cm-3
e- is free to move about the crystal
(Mobility mn ≈1350cm2/V)
+
11
Donors n-Type Material
•
•
•
•
•
•
•
•
Donors
electrons
ex. Phosphorous (P)
“Donates” an extra e- that can freely
travel around
Leaves behind a positively charged
nucleus (cannot move)
Overall, the crystal is still electrically
neutral
negative carriers)
ND = the concentration of donor
atoms [atoms/cm3 or cm-3]
~1015-1020cm-3
e- is free to move about the crystal
(Mobility mn ≈1350cm2/V)
n-Type Material
+
–
+ –
+ –+
–
+ +
+–
+
–
+ –
+ –
+
–
– + –+
+ –+
–
+ +–
–
+
–
+
–
Shorthand Notation
+ Positively charged ion; immobile
– Negatively charged e-; mobile;
Called “majority carrier”
+ Positively charged h+; mobile;
Called “minority carrier”
12
Acceptors Make p-Type Material
•
•
•
h+
–
•
•
•
•
•
Acceptors
Add atoms with only 3 valenceband electrons
ex. Boron (B)
“Accepts” e– and provides extra h+
to freely travel around
Leaves behind a negatively
charged nucleus (cannot move)
Overall, the crystal is still
electrically neutral
positive carriers)
NA = the concentration of acceptor
atoms [atoms/cm3 or cm-3]
Movement of the hole requires
breaking of a bond! (This is hard,
so mobility is low, μp ≈ 500cm2/V)
13
Acceptors Make p-Type Material
p-Type Material
•
–
+
– +
+
– +–
+
– –
+
+
–
–
+
–
–
+
– +
+
–
–
–
–
+
+
– –+
+
–
+
–
+
Shorthand Notation
– Negatively charged ion; immobile
+ Positively charged h+; mobile;
Called “majority carrier”
– Negatively charged e-; mobile;
Called “minority carrier”
•
•
•
•
•
•
•
Acceptors
Add atoms with only 3 valenceband electrons
ex. Boron (B)
“Accepts” e– and provides extra h+
to freely travel around
Leaves behind a negatively
charged nucleus (cannot move)
Overall, the crystal is still
electrically neutral
positive carriers)
NA = the concentration of acceptor
atoms [atoms/cm3 or cm-3]
Movement of the hole requires
breaking of a bond! (This is hard,
so mobility is low, μp ≈ 500cm2/V)
14
The Fermi Function
The Fermi Function
• Probability distribution function (PDF)
• The probability that an available state at
an energy E will be occupied by an e-
f(E)
1
f E  
1
1 e
E  E f  kT
E  Energy level of interest
Ef  Fermi level
 Halfway point
 Where f(E) = 0.5
k  Boltzmann constant
= 1.38×10-23 J/K
= 8.617×10-5 eV/K
T  Absolute temperature (in Kelvins)
0.5
Ef
E
15
Boltzmann Distribution
If E  E f  kT
f(E)
Then
f E   e

 EE f
 kT
1
0.5
Boltzmann Distribution
• Describes exponential decrease in the
density of particles in thermal equilibrium
• Applies to all physical systems
• Atmosphere  Exponential distribution of gas molecules
• Electronics  Exponential distribution of electrons
• Biology  Exponential distribution of ions
Ef
~Ef - 4kT
E
~Ef + 4kT
16
Band Diagrams (Revisited)
E
EC
Ef
Eg
EV
Band Diagram Representation
Energy plotted as a function of position
EC
 Conduction band
 Lowest energy state for a free electron
 Electrons in the conduction band means current can flow
EV
 Valence band
 Highest energy state for filled outer shells
 Holes in the valence band means current can flow
Ef
 Fermi Level
 Shows the likely distribution of electrons
EG
 Band gap
 Difference in energy levels between EC and EV
 No electrons (e-) in the bandgap (only above EC or below EV)
 EG = 1.12eV in Silicon
0.5
1
f(E)
• Virtually all of the
valence-band energy
levels are filled with e• Virtually no e- in the
conduction band
17
Effect of Doping on Fermi Level
Ef is a function of the impurity-doping level
n-Type Material
E
EC
Ef
EV
0.5
1
f(E)
• High probability of a free e- in the conduction band
• Moving Ef closer to EC (higher doping) increases the number of available
majority carriers
18
Effect of Doping on Fermi Level
Ef is a function of the impurity-doping level
p-Type Material
1  f E 
E
EC
Ef
EV
0.5
1
f(E)
• Low probability of a free e- in the conduction band
• High probability of h+ in the valence band
• Moving Ef closer to EV (higher doping) increases the number of available
majority carriers
19
Equilibrium Carrier Concentrations
n = # of e- in a material
p = # of h+ in a material
ni = # of e- in an intrinsic (undoped) material
Intrinsic silicon
• Undoped silicon
• Fermi level
• Halfway between Ev and Ec
• Location at “Ei”
E
EC
Ef
EV
Eg
0.5
1
f(E)
20
Equilibrium Carrier Concentrations
Non-degenerate Silicon
• Silicon that is not too heavily doped
• Ef not too close to Ev or Ec
Assuming non-degenerate silicon
n  ni e
E f  Ei  kT
p  ni e
Ei  E f  kT
Multiplying together
np  ni
2
21
Charge Neutrality Relationship
• For uniformly doped semiconductor
• Assuming total ionization of dopant atoms
p  n  ND  N A  0
# of carriers
# of ions
Total Charge = 0
Electrically Neutral
22
Calculating Carrier Concentrations
• Based upon “fixed” quantities
• NA, ND, ni are fixed (given specific dopings
for a material)
• n, p can change (but we can find their
equilibrium values)
1
2


ND  N A  ND  N A 
2
n
 
  ni 
2
2




N A  N D  N A  N D 
2
p
 
  ni 
2
2



2
2
1
2
2
ni

n
23
Common Special Cases in Silicon
1. Intrinsic semiconductor (NA = 0, ND = 0)
2. Heavily one-sided doping
3. Symmetric doping
24
Intrinsic Semiconductor (NA=0, ND=0)
Carrier concentrations are given by
n  ni
p  ni
n  p  ni
25
Heavily One-Sided Doping
N D  N A  N D  ni
N A  N D  N A  ni
This is the typical case for most semiconductor applications
If N D  N A , N D  ni (Nondegenerate, Total Ionization)
Then n  N D
2
ni
ND
If N A  N D , N A  ni (Nondegenerate, Total Ionization)
Then p  N A
p
2
n
ni
NA
26
Symmetric Doping
Doped semiconductor where ni >> |ND-NA|
• Increasing temperature increases the
number of intrinsic carriers
• All semiconductors become intrinsic at
sufficiently high temperatures
n  p  ni
27
Determination of Ef in Doped Semiconductor
 ND 
 for N D  N A , N D  ni
E f  Ei  kT ln 
 ni 
 NA 
 for N A  N D , N A  ni
Ei  E f  kT ln 
 ni 
Also, for typical semiconductors (heavily one-sided doping)
n
 p
E f  Ei  kT ln    kT ln  
 ni 
 ni 
[units eV]
28
Thermal Motion of Charged Particles
• Look at drift and diffusion in silicon
• Assume 1-D motion
• Applies to both electronic systems and
biological systems
29
Drift
Drift → Movement of charged particles in response to an external field (typically an
electric field)
E-field applies force
F = qE
which accelerates the charged particle.
However, the particle does not accelerate
indefinitely because of collisions with the lattice
(velocity saturation)
Average velocity
<vx> ≈ -µnEx electrons
< vx > ≈ µpEx holes
µn → electron mobility
→ empirical proportionality constant
between E and velocity
µp → hole mobility
µn ≈ 3µp
E
µ↓ as T↑
30
Drift
Drift → Movement of charged particles in response to an external field (typically an
electric field)
E-field applies force
F = qE
which accelerates the charged particle.
However, the particle does not accelerate
indefinitely because of collisions with the lattice
(velocity saturation)
Average velocity
<vx> ≈ -µnEx electrons
< vx > ≈ µpEx holes
µn → electron mobility
→ empirical proportionality constant
between E and velocity
µp → hole mobility
µn ≈ 3µp
Current Density
J n,drift  mn qnE
J p ,drift  m p qpE
q = 1.6×10-19 C, carrier density
n = number of ep = number of h+
µ↓ as T↑
31
Resistivity
• Closely related to carrier drift
• Proportionality constant between electric field and the total
particle current flow

1
where q  1.602 1019 C
qmn n  m p p 
n-Type Semiconductor
p-Type Semiconductor
1

qm n N D
1

qm p N A
• Therefore, all semiconductor material is a resistor
– Could be parasitic (unwanted)
– Could be intentional (with proper doping)
• Typically, p-type material is more resistive than n-type
material for a given amount of doping
• Doping levels are often calculated/verified from resistivity
measurements
32
Diffusion
Diffusion → Motion of charged particles due to a concentration gradient
• Charged particles move in random directions
• Charged particles tend to move from areas of high concentration to areas of
low concentration (entropy – Second Law of Thermodynamics)
• Net effect is a current flow (carriers moving from areas of high concentration
to areas of low concentration)
dn x 
dx
dp  x 
  qD p
dx
J n ,diff  qDn
J p ,diff
q = 1.6×10-19 C, carrier density
D = Diffusion coefficient
n(x) = e- density at position x
p(x) = h+ density at position x
→ The negative sign in Jp,diff is due to moving in the opposite direction
→ The positive sign from Jn,diff is because the negative from the ecancels out the negative from the concentration gradient
33
Total Current Densities
Summation of both drift and diffusion
J n  J n ,drift  J n ,diff
dnx 
dx
 m n qnE  qDnn
 m n qnE  qDn
(1 Dimension)
(3 Dimensions)
J p  J p ,drift  J p ,diff
dpx 
 m p qpE  qD p
dx
 m p qpE  qD p p
(1 Dimension)
(3 Dimensions)
Total current flow
J  Jn  J p
34
Einstein Relation
Einstein Relation → Relates D and µ (they
are not independent of each other)
D
kT

m
q
UT = kT/q
→ Thermal voltage
= 25.86mV at room temperature
≈ 25mV for quick hand approximations
→ Used in biological and silicon applications
35
Changes in Carrier Numbers
Primary “other” causes for changes in carrier concentration
• Photogeneration (light shining on semiconductor)
• Recombination-generation
Photogeneration
n
p

 GL
t light t light
Photogeneration rate
Creates same # of e- and h+
36
Changes in Carrier Numbers
Indirect Thermal Recombination-Generation
p
t

 p
R G
p
n
 n

t R G
n
h+ in n-type material
n0, p0
n, p
Δn, Δp
e-
in p-type material
 equilibrium carrier concentrations
 carrier concentrations under
arbitrary conditions
 change in # of e- or h+ from
equilibrium conditions
Assumes low-level injection
p  n0 ,
n  n0
in n - type material
n  p0 ,
p  p0
in p - type material
37
Minority Carrier Properties
Minority Carriers
• e- in p-type material
• h+ in n-type material
• τn  The time before minority carrier electrons undergo recombination
in p-type material
• τp  The time before minority carrier holes undergo recombination in
n-type material
Diffusion Lengths
• How far minority carriers will make it into “enemy territory” if they are
injected into that material
Ln  Dn n
for minority carrier e- in p-type material
L p  D p p
for minority carrier h+ in n-type material
38
Equations of State
• Putting it all together
• Carrier concentrations with respect to time (all processes)
• Spatial and time continuity equations for carrier concentrations
n n
n
n
n




t t drift t diff t R G t other
( light)

1
  Jn
q




n
n

t R G t other
( light)
Related to Current
p p
p
p



t t drift t diff t
1
p
   Jp 
q
t



R G

R G
p
t other
( light)
p
t other
( light)
Related to Current
39
Equations of State
Minority Carrier Equations
• Continuity equations for the special case of minority carriers
• Assumes low-level injection
n p
t
 Dn
 2 n p
x
2

n p
n
 GL
Light generation
Indirect thermal recombination
J, assuming no E-field
qDn
J
n
1
and also   J n  Dn n
x
q
x
pn
 2 pn pn
 Dn

 GL
2
t
x
p
np, pn  minority carriers in “other” type of material
40
```
Related documents